Journal of Crystal Growth 317 (2011) 1–3
Contents lists available at ScienceDirect
Journal of Crystal Growth journal homepage: www.elsevier.com/locate/jcrysgro
Czochralski growth of a-BBO crystals under azimuthally anisotropic heating$ Konstantin Kokh n, Alexander Kokh Institute of Geology and Mineralogy SB RAS, Novosibirsk, Russia
a r t i c l e in f o
Presented at the Romanian Conference on Advanced Materials—ROCAM 2009, August 25–28, 2009, Brasov, Romania Available online 18 November 2010
Crystal growth of a-BBO in a modiﬁed low-gradient Czochralski furnace was performed. The distribution of temperature inside the furnace was described by a three-fold symmetry axis (L3). The axial temperature gradient under the melt was 2 K/cm, while that inside the melt was almost equal to zero. A 36 mm thick sample of the grown crystal shows extremely low 0.05 cm 1 absorption coefﬁcient at wavelengths 4220 nm. & 2010 Elsevier B.V. All rights reserved.
Keywords: A1. Heat ﬁeld symmetry A2. Growth from melts B1. Borates
1. Introduction BaB2O4 (BBO) crystals are well known NLO materials due to
b-modiﬁcation existing below 925 1C . But the structure of a-phase has a center of symmetry, which disables the nonlinear properties. On the other hand, a big transparency region (189–3500 nm) and high birefringence of a-phase crystals provide good materials to substitute calcite, TiO2, LiNbO3, etc. Since BBO melts congruently, the easiest way for crystal growth seems to be a classical Czochralski method. Because of the high
melt viscosity one should impose high gradients of temperature during crystal growth. Therefore crystallization from the stoichiometric melts often results in thermal stresses  and spontaneous a–b phase transition [3,4] in the grown crystals. One of the ways to solve the problem of melt viscosity is the use of high temperature solutions. Addition of a solvent like Na2O, PbO, etc. decreases both viscosity and crystallization temperature . But solution growth of a-BBO results in the formation of microinclusions in the bulk. Therefore the main disadvantage of this technique is a low yield of the material.
Fig. 1. Sketch of heater (a); ﬂow pattern on surface of melt (b); and surface of frozen melt after growth experiment (c).
$ Presented at the Romanian Conference on Advanced Materials – ROCAM 2009, August 25–28, 2009, Brasov, Romania. n Corresponding author. Tel./fax: +7 383 3333947. E-mail address: [email protected]
0022-0248/$ - see front matter & 2010 Elsevier B.V. All rights reserved. doi:10.1016/j.jcrysgro.2010.11.027
K. Kokh, A. Kokh / Journal of Crystal Growth 317 (2011) 1–3
2. Experimental details A main modiﬁcation of the Czochralski furnace consists of nonuniform heating of the crystallization medium. The heater framework is composed of an alumina pipe cut into three 1001 sectors (Fig. 1a). Ceramic blocks are wrapped with a resistive wire and the sectors are connected serially outside the hot zone. Gaps among the sectors are in turn ﬁlled with caoline wool to increase the anisotropy of crucible heating. In this way the crucible walls are heated by three ‘‘hot’’ areas giving rise to a speciﬁc pattern of natural convection (Fig. 1b). Observation of the melt surface reveals three dark rays indicating areas of more cold descending ﬂows. Each ray begins at the corresponding ‘‘gap between heaters’’ and extends to the center of the crucible. Thus the convective structure inherits the symmetry of the heat ﬁeld and is likely to be explained by the existence of three separate vortices positioned between the dark rays. One of the features of the Czochralski method is a constantly decreasing melt level; so it is a problem to maintain the convective structure during the crystal growth. In this work a single crystal on
the frozen surface is observed after every experiment (Fig. 1c). Orientation of the crystal marks the directions of the dark rays seen before the start of the experiment. Therefore the stability of convection is assumed to be sufﬁciently high. Fig. 2 shows the temperature distribution measured by an S-type thermocouple along the central axis. The temperature gradient above the melt surface is about 2 K/cm while that inside the melt is almost equal to zero except at the near-surface region. It should be noted that these thermal conditions are quite unusual for crystal growth from a viscous melt. For instance, the authors of Ref.  grew a-BBO crystals with a 70–80 1C temperature difference in the melt along the central axis.
3. Growth of a-BBO crystals Crystal growth of a-BBO was performed in the modiﬁed lowgradient Czochralski furnace. Solid state synthesis of the charge was done at 800 1C from BaCO3 (3 N) and HBO2 (3 N). The stoichiometric charge was melted in Ø80 mm crucible. The furnace was put on the balance sensor in order to provide automatic control of crystal diameter with feedback ratio 0.8 1C per 1 g. Other growth parameters were as follows: seed orientation— (0 0 0 1), crystal pulling—5 mm/day, and crystal rotation—4 rpm. The cooling rate after growth was 20 K/h. Fig. 3a presents a photo of the as-grown crystal. The typical weight of the crystals is 300 g. All crystals exhibit well-developed rhombohedra facets. The convex front of crystallization has a small plateau of the (0 0 0 1) plane at the center. Fig. 3b shows a slice of the a-BBO crystal polished perpendicular to the growth direction. The central part of the crystal demonstrates a defect region with the swirl structure (marked by the dash) but the other part of the crystal exhibits high optical quality. An absorption spectrum of the high-quality part of the 36 mm width sample is presented in Fig. 3c. The absorption coefﬁcient at wavelengths 4 220 nm corresponds to an extremely low value of 0.05 cm 1.
Fig. 2. Measured temperature distribution along central axis.
It was shown that growth of high-quality a-BBO crystals is possible under low temperature gradients. The temperature
Fig. 3. As-grown a-BBO crystal (a) and polished slice (b) 36 mm in width, with cell size of 5 5 mm2. (c) Absorption spectra of a-BBO sample at room temperature.
K. Kokh, A. Kokh / Journal of Crystal Growth 317 (2011) 1–3
inhomogeneties imposed to the melt are supposed to play an important role in convection processes in the growing crystal. Hence the proposed technique seems to be promising for crystal growth from viscous melts.
Acknowledgement This work is supported by the VMTK2009N5 grant.
References  V.G. Dmitriev, G.G. Gurzadyan, D.N. Nicogosyan, Handbook of Nonlinear Optical Crystals, Springer-Verlag, New York, 1999.  V.P. Solntsev, E.G. Tsvetkov, V.A. Gets, V.D. Antsygin, Growth of a-BaB2O4 single crystals from melts at various compositions: comparison of optical properties, J. Cryst. Growth 236 (2002) 290–296.  S. Wu, G. Wang, J. Xie, X. Wu, Y. Zhang, X. Lin, Growth of large birefringent a-BBO crystal, J. Cryst. Growth 245 (2002) 84–86.  J. Liu, X. He, J. Xu, G. Zhou, S. Zhou, G. Zhao, S. Li, The study on properties of Sr2 + doped a-BBO crystal, J. Cryst. Growth 260 (2004) 486–489.